• Study Resource
• Explore

Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Document related concepts

X-ray fluorescence wikipedia, lookup

Diffraction grating wikipedia, lookup

Phase-contrast X-ray imaging wikipedia, lookup

Powder diffraction wikipedia, lookup

Low-energy electron diffraction wikipedia, lookup

Anti-reflective coating wikipedia, lookup

Diffraction topography wikipedia, lookup

Airy disk wikipedia, lookup

Reflection high-energy electron diffraction wikipedia, lookup

Nonlinear optics wikipedia, lookup

Rutherford backscattering spectrometry wikipedia, lookup

Upconverting nanoparticles wikipedia, lookup

X-ray crystallography wikipedia, lookup

Transcript
```Chapter 2: Wave Diffraction &
The Reciprocal Lattice (continued)
Chapter Topics
1. Wave Diffraction by Crystals
2. Bragg Law
3. Scattered Wave Amplitude
4. Reciprocal Lattice
5. Brillouin Zones
6. Fourier Analysis of the Basis
Diffraction of Waves by Crystalline Solids
• We know that a crystal is a periodic structure with unit
cells that are repeated regularly.
Crystal Structure Information
can be obtained by understanding the diffraction
patterns of waves (of appropriate wavelengths)
interacting with the solid. Analysis of such diffraction
patterns is a main topic of this chapter.
It is common to study crystal structures with
X-rays, Neutrons & Electrons.
Of course, the general principles are the same for each type of wave.
• The results of crystal diffraction depend on the
crystal structure and on the wavelength.
• At optical wavelengths such as 5,000 Ǻ, the
superposition of waves scattered elastically by
the individual atoms of a crystal
results in ordinary optical refraction.
• When the wavelength of the radiation is
comparable to or smaller than the lattice
constant, diffracted beams occur in
directions quite different from the direction
Wavelength vs Energy
Quantum Mechanical Result
The energy & momentum of a
particle with De Broglie
Wavelength λ are
E = (hc/λ) & p = (h/ λ)
(h = Planck’s constant)
Diffraction from crystal planes
requires λ to be of the same
order of magnitude as the
distance d between planes:
d  a few Ångstroms
so λ must also be in that range.
This gives
Photons: E  keV
Neutrons: E  0.01 eV
Electrons: E  100 eV
Typical X-Ray Experiment & Data
X-Ray Diffraction Resultsfor Powdered Si
(Relative Intensities are Due to the 2 Atom Basis.)
Monochromator
• Crystal Structure can be found by studying the Diffraction
Pattern of a beam of radiation incident on the crystal.
• Beam diffraction takes place only in certain specific
directions, much as light is diffracted by a grating.
• By measuring the directions of the diffraction and the
corresponding intensities, information about the Crystal
Structure responsible for the diffraction.
X-Ray Diffraction
• W.H. & W.L. Bragg (father & son!) were the first
to develop a simple explanation of the X-Ray
diffracted beams from a crystal.
• The Bragg derivation is simple but it is convincing
since only it reproduces the result that agrees with
observations.
X-Ray Diffraction & The Bragg Equation
• English physicists Sir W.H. Bragg
& his son W.L. Bragg developed
a theory in 1913 to explain why the
cleavage faces of crystals
appear to reflect X-rays
ONLY at certain angles of
incidence θ.
This is an example of
X-Ray Diffraction
Sir William H. Bragg
(1862-1942)
Sir William L. Bragg
(1890-1971)
In 1915, the father & son were awarded the Nobel prize in physics
“For their services in the analysis of
crystal structure by means of X-Rays".
(The younger Bragg was fighting in WWI when he received the Nobel Prize!)
Crystal Structure Determination
A Crystal behaves as a 3-D
Diffraction Grating for X-Rays
• In a diffraction experiment, the spacing of lines on
the grating can be found from the separation of the
diffraction maxima. Also, information about the
structure of the lines on the grating can be obtained
by measuring the relative intensities of different orders
• Similarly, measurement of the separation of the XRay diffraction maxima from a crystal enables the
determination of the unit cell size. Also, from the
intensities of diffracted beams, information can be
obtained about the arrangement of atoms within the cell.
X-Ray Crystallography
• For X-Rays, the wavelength λ
is typically  a few Ångstroms,
which is comparable to the
interatomic spacing (distances
between atoms or ions) in crystals.
• So, for crystal structure
determination, the X-Rays
have to be of energy:
hc
hc
3
Exray    h  
 12.3x10 eV
10
 1x10 m
Bragg Law
• Consider crystals as made up of parallel planes of
atoms. Incident waves are reflected specularly from
parallel planes of atoms in the crystal, with each
plane reflecting only a very small fraction of the
radiation, like a lightly silvered mirror.
• In mirrorlike reflection, the angle of incidence is
equal to the angle of reflection.
ө
ө
Diffraction Condition
• The diffracted beams are found to have maximum intensity when the
Reflections from Planes of Atoms
Interfere Constructively.
Assume elastic scattering, in which the X-Ray energy isn’t changed on reflection.
• So, when X-Rays strike a crystal, we want the condition for
constructive interference between reflected rays from different planes.
That is, we want the condition for the reflected X-rays to be inphase with one another so that they that add together constructively.


2
Incident Angle  θ
Reflected angle  θ
X-ray Wavelength  λ
Total Diffracted
Angle  2θ
Bragg Law
• The two X-Ray beams travel different distances. The difference in the
distances traveled is related to the distance between the adjacent layers.
• See Figure. Connecting the two beams with perpendicular lines shows
the difference in the distance traveled between top & bottom beams.
• In the figure, the length DE is the same as EF, so the total distance
traveled by the bottom wave is expressed by:
• Constructive interference of the radiation from successive planes
occurs when the path difference is an integral number of wavelengths.
• Note that line CE = d = distance between the 2 layers
• So: DE  d sin  EF  d sin  DE  EF  2d sin 
• Giving: n  2d sin  This is called the Bragg Law
Bragg Law (Bragg Equation)
2d sin   n
d = Spacing of the Planes
n = Order of Diffraction.
• Because sin θ ≤ 1,
Bragg reflection can only occur for
wavelengths satisfying: n  2d
• This is why visible light can’t be used. No diffraction
occurs when this condition is not satisfied.
• The diffracted beams (reflections) from any set of
lattice planes can only occur at particular angles
predicted by Bragg’s Law.
• Now, a similar, but slightly different treatment:
• See Figure: Consider X-Rays incident at angle θ
on one of the lattice planes. Look at the
Scattering of these X-Rays from
• There will be Constructive Interference of the
waves scattered from the two successive lattice points A
& B in the plane if the distances AC and DB are equal.
D
C

A
2
B
So, look at the conditions for
Constructive Interference
of Waves Scattered from the same plane.
• If the scattered wave makes the same angle with the
plane as the incident wave (see figure on the previous slide):
The diffracted wave will look as if it was reflected from the plane.
• It is common to consider
Scattering from Lattice Points Rather than Atoms
because it is the basis of atoms associated with each
lattice point that is the true repeat unit of the crystal.
• The lattice point is an analogue of the line on an optical diffraction
grating. The basis represents the structure of the line.
Diffraction Maxima
• Coherent scattering from a single plane is not sufficient
to obtain a diffraction maximum. It is also necessary
That Successive Planes also
Scatter in Phase.
• This will be the case if the path difference for
scattering off of two adjacent planes is an
integral number of wavelengths. That is, if
2d sin   n
• Although the reflection from each plane is
specular,
Only for certain values of  will the
reflections from all planes add up in
phase to give a strong reflected beam.
• Each plane reflects only 10-3 to 10-5 of the
incident radiation, i.e. it is not a perfect reflector.
• So, 103 to 105 planes contribute to the formation
of the Bragg-reflected beam in a perfect crystal.
• The composition of the basis determines the relative
intensity of the various orders of diffraction.
Scattered Wave Amplitude 
Reciprocal Lattice Vectors
• Now, consider X-Ray Scattering from
crystals & analyze the
Amplitude of the Scattered Waves.
• The electronic number density n(r) in the
crystal is a periodic function in space:
n(r) = n(r +T)
with period T equal to a
Direct Lattice Translation Vector:
T = n1a1 + n2a2 + n3a3
• The electronic number density n(r) in the crystal is
periodic in space: n(r) = n(r +T), with T equal to a
Direct Lattice Translation Vector:
T = n1a1 + n2a2 + n3a3
• So, n(r) can be expressed as a (spatial) Fourier series
expansion. So, for a one-dimensional model crystal, n(x)
can be represented as


n( x)  n0   C p cos( 2px / a)  S p sin( 2px / a)   n p ei 2px / a
p 0
p
where the p’s are integers and the Fourier coefficient of
the number density can be written as:
a
n p  1a  dxn( x)e i 2px / a
0
• In 3 Dimensions, the Fourier coefficient of the
number density has the form:
n(r )   nG e
iG r
G
a
 nG  V1  dVn (r )e iG r
c
0
(1)
The vectors G are called
Reciprocal Lattice Vectors
• As we said, the electronic density n(r) is required
to be invariant (periodic) under lattice translations:
n(r) = n(r +T)
(2)
• That is, it must satisfy:
n(r  T)   nG eiG(r T)   nG eiGr eiGT  n(r ) when eiGT  1
G
G
(3)
• Only The Set of Reciprocal Lattice Vectors G that
satisfy both (1) & (3) (previous slide) lead to an electronic
number density n(r) that is invariant under lattice translations.
• It’s not too hard to show that the set of G’s that meet this
requirement are of the form
G  v1b1  v2b 2  v3b3
where υ1, υ2 & υ3 are integers & the bi’s are vectors
which are defined as:
b i  2
a j  ak
ai  a j  a k 
, i  x, y, z  bi  a j  2ij
• The aj’s are the primitive lattice vectors for the crystal
structure. It also can be shown that
The Set of Reciprocal Lattice Vectors
G is a Bravais Lattice!
The Diffraction Condition (Bragg’s
Law) in the Reciprocal Lattice
• An X-Ray diffraction pattern of the lattice
Can be interpreted as a map of the
reciprocal lattice of the crystal.
This statement is consistent with the following theorem:
The Set of Reciprocal Lattice
Vectors G determines
the possible X-ray reflections.
• An X-Ray diffraction pattern of the lattice
Can be interpreted as a map of the
reciprocal lattice of the crystal.
In other words
The Set of Reciprocal Lattice Vectors G
determines the possible X-ray reflections.
Wavevector Representation
of X-ray Scattering: k  k´
F   dVn(r )ei (k k')r
r
d
The scattered wave
amplitude is:
w
  dVn(r )e ik r
k
k´
When G = k (wavevector),
then F = V nG.
• Now, look at this condition for elastic
scattering (specular reflection):
2
G  k  k'k  2k  G  G  0
This result is called
The Laue Condition.
It’s not too difficult to show that
it is 100% equivalent to
The Bragg Law!
The Laue Condition is:.
2
G  k  k'k  2k  G  G  0
This is 100% equivalent to The Bragg Law!
The result that k = G can also be expressed to give the relations that
are called The Laue Relations or the Laue Equations. These are
obtained by taking the dot product of both Δk & G with
a1, a2 & a3. The Laue Equations are: k  ai  2vi , i  1,2,3
By changing θ, X-Ray diffraction
can be used to map all
 k´ 2θ
k
G
Reciprocal Lattice Vectors.
This geometric method of finding
Reciprocal Lattice Vectors is called
The Ewald Construction
Brillouin Zones & Reciprocal Lattices
for the SC, BCC & FCC Lattices
Brillouin Zones
The First Brillouin Zone (BZ) is defined as the WignerSeitz primitive cell in the reciprocal lattice. It gives a geometric
interpretation, in the reciprocal lattice, of the diffraction condition.
• The Brillouin construction exhibits
all wavevectors k that can be
Bragg reflected
by the crystal.
• The constructions divide the
reciprocal space into fragments, out
of which
The First Brillouin Zone
is of the greatest importance.
Reciprocal Lattices for the SC, FCC & BCC Lattices
Direct Lattice
Reciprocal Lattice
Volume
SC
FCC
BCC
 a1  ax

a 2  ay
a  az
 3
 b1  2 / a x

b 2  2 / a y
b  2 / a z
 3
2 / a 3
 a1  1 ax  y 
2

1 a y  z 
a

 2 2
 a  1 a z  x 
 3 2
b1  2  x  y  z 
a

2 x  y  z 
b

 2 a
b  2 x  y  z 
 3 a
22 / a 3
a1  1 ax  y  z 
2

1 a  x  y  z 
a

 2 2
a  1 ax  y  z 
 3 2
 b1  2 y  z 
a

2 x  z 
b

 2 a
b  2 x  y 
 3 a
42 / a 3
Brillouin Zones: Square Lattice
First 4 Brillouin Zones: Square Lattice
“All” Brillouin Zones: Square Lattice??
First Brillouin Zone: BCC Lattice
First Brillouin Zone: FCC Lattice
Reciprocal Lattice for Aluminium
Fourier Analysis of a Basis
Structure Factor & Atomic Form Factor.
• Earlier, we said that the scattering amplitude for a unit
cell has the form:
F   dVn (r)e iGr  NSG
cell
The quantity SG is called The Structure Factor. It is defined
as an integral over a single unit cell. If the electron density is
written as a superposition of the electron densities in the cell,
taking into account the # of atoms in the basis, it has the form:
s
n(r )   n j (r  r j )
j 1
where s is the # of atoms in the unit cell.
Using this, The Structure Factor has the form:
s
SG    dVn j (r  r j )e iGr
j 1 cell
s
 e
iG r j
j 1
 dVn j ()e
cell
iG 
s
 e
j 1
iG r j
fj
The quantity fj is called The Atomic Form Factor.
Now specifying G and rj as
G  v1b1  v2b 2  v3b3 and r j  x j a1  y j a 2  z j a3
gives:
s
SG   f j e
 2 i x j v1  y j v2  z j v3 
j 1
Note that SG can be complex, because the scattering
intensity involves the magnitude squared of SG.
• If (& only if!) the electron density of the
atom is spherically-symmetric, the atomic
form factor fj can be written:

f j  4  n j ( r ) r
2 sin Gr 
dr
Gr
0
This means that when the electronic density has the form
n(r) = Zg(r), then fj = CZ
(C = constant, Z = atomic charge,)
That is, in this case, fj is the ratio of radiation
amplitude scattered by the electron distribution
to that scattered by a localized electron.
Examples of Structure Factor Calculations
BCC lattice
In a BCC lattice, there are 2 atoms per cubic unit cell
located at (000) & (½½ ½). The structure factor is then:

SG  1  e
i v1 v2 v3 
f
This structure factor has its Maximum, SG = 2f
when the sum of the indices is even. That is when:
υ1+ υ2+ υ3 = 2n (n = integer)
This structure factor Vanishes, SG = 0 when the
sum of the indices is odd. That is when:
υ1+ υ2+ υ3 = 2n + 1
(n = integer)
Examples of Structure Factor Calculations
FCC lattice
For a FCC lattice, there 4 atoms per cubic unit cell
located at (000), (0½½), (½ 0½) & (½½0). The structure
factor is then:

SG  1  e
i v1 v2 
e
i v1 v3 
e
i v2 v3 
f
This structure factor has its Maximum, SG = 4f
when all indices υ1, υ2, υ3 are even or odd,
This structure factor Vanishes, SG = 0 when the
indices are partially even & partially odd.
To summarize, in a FCC lattice, no reflections occur
when the indices are partially even and partially odd.
Observed & Calculated
Atomic Form Factor for Aluminium
From Ch. 1:
Lattice Planes & Miller Indices
• A Lattice Plane is any plane containing at least
three non-colinear Bravais lattice points.
• Generally, a lattice plane is described by giving a
vector normal to that plane, & there happens to be
reciprocal lattice vectors normal to any lattice plane.
• Choose the the shortest such reciprocal lattice
vector to arrive at the Miller indices of the plane.
• Thus a plane with Miller indices h, k, l, is normal
to the reciprocal lattice vector hb1 + kb2 + lb3.
Review of Miller Indices Continued
Imagine representing a crystal structure on a grid
(lattice) which is a 3D array of points (lattice
points). Now, imagine dividing the grid into sets
of “planes” in different orientations:
Review of Miller Indices Continued
Recall That
• All planes in a set are identical.
• The perpendicular distance between pairs of
• Miller Indices define the orientation of the plane
within the unit cell.
• The Miller Indices define a set of planes parallel
to one another: (002) planes are parallel to (001)
planes, and so on.
• So, in analyzing crystal diffraction results, the
lattice planes are labeled with their Miller
Indices (hkl) for their identification.
Labelling the Reflection Planes
Label reflections with the Miller
indices of the planes.
• A beam corresponding to a diffraction order of n >1
could be identified by a statement such as
“The nth-order reflections from the (hkl) planes”
or a
“(nh nk nl) reflection”.
p
Example
A 3rd order reflection from the (111) plane is
“a (333) reflection”
nth Order Diffraction Off of (hkl) Planes
• Rewrite the Bragg Law in the form:
d 
2
 sin   
 n
l
• This makes
the nth order diffraction off of (hkl)
planes of spacing “d” look like
the 1st order diffraction off planes of
spacing (d/n).
• Planes of this reduced spacing would have
Miller indices (nh nk nl).
X-Ray Structure Analysis of NaCl & KCl
General Prıncıples of X-Ray Structure Analysıs
Applied to Find the Crystal Structures
of NaCl & KCl
• The Braggs measured the intensity of specular reflection
from cleaved faces of NaCl & KCl crystals.
• They found 6 values of θ for which a sharp peak in
intensity occurred, corresponding to 3 characteristic
wavelengths (K,L and M X-Rays) in 1st & 2nd order (n = 1
& n = 2 in the Bragg Law)
• By repeating the experiment with a different crystal face
they could use the Bragg Equation to find, for example, the
ratio of (100) & (111) plane spacings, information that
confirmed the cubic symmetry of the atomic arrangement.
Details of the Structure
• Details of the crystal structure were then found. They
also discovered some surprising differences between the
diffraction patterns for NaCl and KCl.
A Major Difference
was the absence of (111) reflections in
KCl compared to weak but detectable
(111) reflections in NaCl.
• The explanation for this is that the K and
Cl ions both have the argon electron shell
structure and hence scatter x-rays almost
equally. However, the Na and Cl ions
have very different scattering strengths.
The (111) reflection in NaCl corresponds
to a one wavelength path difference
between neighboring (111) planes.
Measurement Results
XRD Pattern
for NaCl
XRD Pattern
for KCl
d - Spacing Formula
d ≡ Distance between Parallel Lattice
Planes with Miller Indices (hkl)
Its not difficult to prove the following:
Orthogonal
Cubic
Crystal Systems
( =  =  = 90)
Crystal Systems
(a = b = c)
2
2
2
1 h
k
l
 2 2 2
2
d
a
b
c
1 h k l

2
2
d
a
2
2
2
A cubic crystal system is a special case of an
orthogonal crystal system.
Bragg Equation
• Since Bragg's Law applies to all sets of crystal planes,
the lattice structure can be found from the diffraction
pattern, making use of general expressions for the
spacing of the planes in terms of their Miller
indices (hkl), along with the Bragg Law.
• For cubic structures:
2d sin   n
d
a
h k l
• Note that the smaller the spacing, the higher the
angle of diffraction, i.e. the spacing of peaks in the
2
2
2
diffraction pattern is inversely proportional to the
spacing of the planes in the lattice. The diffraction
pattern will reflect the symmetry properties of the lattice.
Some Results for d-2
For Some Non-Cubic Lattices
Bragg Equation
• A simple example is the difference between the
series of (n00) reflections for a simple cubic
and a body centred cubic lattice. For the simple
cubic lattice, all values of n will give Bragg peaks.
• However, for the body centered cubic lattice the
(100) planes are interleaved by an equivalent set at
the halfway position. At the angle where Bragg's
Law would give the (100) reflection the interleaved
planes will give a reflection exactly out of phase
with that from the primary planes, which will
Exactly cancel the signal.
• So, in the BCC lattice, there is no signal from (n00)
planes with odd values of n. This kind of argument
leads to rules for identifying the lattice symmetry from
"missing" reflections, which are often quite simple.
Another (Equivalent) Treatment
of The Reciprocal Lattice
• From another internet source. Slightly different notation, sorry!
• Suppose we have a Bravias Lattice, with translational
vector R, & a plane wave, eik·r. Generally, for a given k,
the plane wave will not have the periodicity of the
Bravais lattice, R. However,
for a given R, there will be a set of wave
vectors, K, that will yield plane waves with
the periodicity of the Bravais lattice.
eiK·r = eiK·(r + R) = eiK·r eiK·R
thus,
eiK·R = 1 or K·R = 2nπ
The Reciprocal Lattice
• The Reciprocal lattice is a Bravais lattice.
A brief proof:
bi = 2π(aj × ak )/(ai • aj × ak) then bi • aj = 2 π δij.
Furthermore, any vector, k, can be written as
k = k1b1 + k2b2 + k3b3.
For any vector in the direct lattice, R,
k • R = 2 π(k1n1 + k2n2 + k2n2 ),
so for eik • R to be unity for all R, k • R must be 2π times an
integer n. So the coefficients ki must also be integers.
Therefore, the set of Reciprocal
Lattice Vectors, K are themselves a
Bravais lattice
The Reciprocal Lattice:
• The reciprocal lattice of the reciprocal lattice?
• It is just the direct lattice!
Brillouin Zone
• Brillouin Zones are primitive cells that
arise in the theories of electronic levels
Band Theory &
Lattice Vibrations - Phonons.
• The first Brillouin Zone (BZ) is the WignerSeitz primitive cell of the reciprocal lattice.
Another (Equivalent) Treatment
Von Laue Formulation of Crystal Diffraction
• From another internet source. Slightly different notation, sorry!
• Doesn’t assume specular reflection.
• No sectioning by planes
• Rather, at each point on the Bravais lattice the
incident ray is allowed to be scattered in all directions
First, consider only two scatterers.
k = kn
k´ = kn´
θ
d
θ´
The path difference is then
d cosθ + d cosθ´ = d • (n - n´)
k = 2πn/λ
k´ = 2πn´/λ
The condition for constructive
interference is,
d • (n - n´) = mλ
• With an array of scatterers; one at each point of the
Bravais lattice,
• The results on the last slide must hold for each d that is a
Bravais lattice vector, so
R•(k - k´) = 2πm
(m = integer) or
eiR•(k - k´) = 1!!
• Compare this to the definition for the reciprocal lattice!
This is just The Laue Condition:
Constructive interference will occur
provided that the change in wave vector,
K = k´ - k, is a vector in the reciprocal lattice.
Ewald Construction
• The condition for constructive interference is that
K = k´ - k, is a vector of the reciprocal lattice.
Doing this for all k & k´ generates the Reciprocal Lattice
```
Related documents